Description

A general procedure to evaluate many-body spin operator amplitudes from periodic calculations: application to cuprates

All materials on our website are shared by users. If you have any questions about copyright issues, please report us to resolve them. We are always happy to assist you.

Related Documents

Share

Transcript

This content has been downloaded from IOPscience. Please scroll down to see the full text.Download details:IP Address: 80.193.214.226This content was downloaded on 17/10/2013 at 06:50Please note that terms and conditions apply.
A general procedure to evaluate many-body spin operator amplitudes from periodiccalculations: application to cuprates
View the table of contents for this issue, or go to the journal homepage for more
2007 New J. Phys. 9 369(http://iopscience.iop.org/1367-2630/9/10/369)HomeSearchCollectionsJournalsAboutContact usMy IOPscience
The open–access journal for physics
New Journal of Physics
A general procedure to evaluate many-bodyspin operator amplitudes from periodiccalculations: application to cuprates
Ibério de P R Moreira
1
,
4
, Carmen J Calzado
2
, Jean-Paul Malrieu
3
and Francesc Illas
1
1
Departament de Química Física and Institut de Química Teòrica iComputacional (IQTCUB), Universitat de Barcelona and Parc Cientíﬁc deBarcelona, C
/
Martí i Franquès 1, E-08028 Barcelona, Spain
2
Departamento de Química Física, Universidad de Sevilla, C
/
Prof. GarcíaGonzález s
/
n, E-41012 Sevilla, Spain
3
IRSAMC, Laboratoire de Physique Quantique, Université Paul Sabatier,118 Route de Narbonne, F-31062 Toulouse-Cedex, FranceE-mail: i.moreira@ub.edu, francesc.illas@ub.edu, calzado@us.es and
malrieu@irsamc.ups-tlse.fr
New Journal of Physics
9
(2007) 369
Received 18 May 2007Published 12 October 2007Online at http://www.njp.org/
doi:10.1088/1367-2630/9/10/369
Abstract.
A general procedure is presented which permits the form of anextended spin Hamiltonian to be established for a given magnetic solid andthe magnitude of its terms to be evaluated from spin polarized, Hartree–Fock or density functional calculations carried out for periodic models. Thecomputational strategy makes use of a general mapping between the energyof pertinent broken-symmetry solutions and the diagonal terms of the spinHamiltonian in a local representation. From this mapping it is possible todeterminenotonlytheamplitudeofthewell-knowntwo-bodymagneticcouplingconstants between near-neighbor sites, but also the amplitudes of four-bodycyclicexchangeterms.Ascrutinyoftheon-sitespindensitiesprovidesadditionalinformation and control of the many broken-symmetry solutions which can befound. The procedure is applied to the La
2
CuO
4
, Sr
2
CuO
2
F
2
, Sr
2
CuO
2
Cl
2
andCa
2
CuO
2
Cl
2
square lattices and the SrCu
2
O
3
ladder compound. It is shown thata proper description of the magnetic structure of these compounds requires thattwo- and four-body terms are explicitly included in the spin Hamiltonian. Theimplications for the interpretation of recent experiments are discussed.
4
Author to whom any correspondence should be addressed.
New Journal of Physics
9
(2007) 369 PII: S1367-2630(07)50628-2
1367-2630/07/010369+25$30.00 © IOP Publishing Ltd and Deutsche Physikalische Gesellschaft
2
Contents
1. Introduction 22. Theoretical background and methodology 63. Computational details 134. Results 14
4.1. Spin Hamiltonian parameters for the 2D square lattices . . . . . . . . . . . . . 144.2. Spin Hamiltonian parameters for the SrCu
2
O
3
spin ladder compound . . . . . . 174.3. Critical analysis of the results . . . . . . . . . . . . . . . . . . . . . . . . . . . 19
5. Summary, conclusions and possible extensions 21Acknowledgments 23References 23
1. Introduction
The discovery of the anomalous properties of high-
T
c
superconducting cuprates (HTCSs) inthe late eighties has triggered a considerable interest in the crystal and electronic structure of these compounds from both experimental and theoretical points of view [1]–[5]. An enormous
research effort on ceramic materials, mostly based on copper oxides, has been carried outcontinuously to try to improve the properties of known structures and synthetic pathways andhas resulted in the synthesis of a wide variety of cuprates. The impressive richness of low-dimensional magnetic behavior of the different copper compounds can be, to a large extent,traced back to the stacking of the distorted CuX
6
octahedra (or CuX
5
pyramidal or CuX
4
planarunits) in the lattice [4, 6]. Most of the cuprate based materials are formed by almost independent
CuO
4
units with distant apical ligands to complete the strongly distorted CuO
4
X
2
or CuO
4
Xunits and, hence, the structure is dominated by the link between CuO
4
units. Depending onthe nature of the counter ions and on the number of links between the different CuO
4
units,different structures can be formed ranging from the typical lamellar two-dimensional (2D)structure of the HTCSs to many lower dimensional structures by different combinations of edge-sharing and corner-sharing CuO
4
plaquettes (or CuO
4
units) that can give rise to spin ladders(e.g. Sr
n
−
1
Cu
n
O
2
n
−
1
series with
n
2 [7]–[9]), zigzag spin chains (e.g. SrCuO
2
[10]) andquasi-1D systems (e.g. A
2
CuO
2
(A
=
Ca,Sr) [11, 12] or Li
2
CuO
2
[13]) formed by edge-sharingCuO
4
units.The electronic ground state of this kind of materials is usually described by the openshell nature of the Cu
2+
ions arranged in the CuO
4
units in which the Cu
(
3d
9
)
atomicconﬁguration gives rise to a d
x
2
–
y
2
type hole with the lobes pointing towards the O ions.The resulting Cu–O–Cu pathways range from
∼
90
◦
to 180
◦
and they are responsible forthe rich variety of low-dimensional magnetic structures dominated by moderate ferromagnetic(FM) to strong antiferromagnetic (AFM) interactions. From the theoretical point of view, thesesystems are strongly correlated in nature, making standard band theory techniques based ondensity functional theory (DFT) unable to accurately describe either their valence or low energyspectrum [14]. However, it has been shown that hybrid exchange-correlation functionals canprovide reliable descriptions of strongly correlated transition metal magnetic systems ([15] andreferences therein).
New Journal of Physics
9
(2007) 369 (http://www.njp.org/ )
3Most of the HTCS materials have a lamellar structure in which strong AFM interactionstake place along 180
◦
Cu–O–Cu bonds in edge sharing Cu
4
O
4
plaquettes leading to a 2Dnetwork of effective spin
S
=
1
/
2 particles. These strong magnetic interactions observed in theHTCS are thought to be fundamental ingredients of the high-
T
c
superconductivity microscopicmechanism [5, 16]. Since these compounds may be regarded as effective
S
=
1
/
2 spin lattices,their low energy spectrum and collective properties are assumed to be governed by a simpliﬁedHeisenberg Hamiltonian as in equation (1)
ˆ
H
=
i
,
j
J
ij
ˆ
S
i
· ˆ
S
j
−
14
,
(1)which only accounts for the magnetic coupling
J
ij
between nearest-neighbor (NN) centers
i
and
j
. This is in agreement with the widely accepted general picture for HTC superconductivityinvolving a ‘Heisenberg sea’ where holes or electrons are introduced by doping the perfectstructures. However, it has been claimed that to fully understand the magnetic excitations,infrared and neutron scattering spectra of 2D [17]–[23] and spin ladder cuprates [24, 25] it
is necessary to extend the spin Hamiltonian as in equation (2)
ˆ
H
=
i
,
j
J
ij
ˆ
S
i
· ˆ
S
j
−
14
+
i
,
j
,
k
,
l
J
ring
ˆ
S
i
· ˆ
S
j
ˆ
S
k
· ˆ
S
l
+
ˆ
S
i
· ˆ
S
l
ˆ
S
j
· ˆ
S
k
−
ˆ
S
i
· ˆ
S
k
ˆ
S
j
· ˆ
S
l
−
116
+
· · ·
.
(2)In this expression the constants 1
/
4 and 1
/
16 have been introduced to deﬁne the zero of energyas that of the FM solution. In this spin model, the signs and amplitudes of the local intersitemagnetic interactions govern the collective properties of a spin lattice. They appear as the basicingredients of the effective spin Hamiltonian which in full generality involves not only thetwo-body exchange
J
ij
but also other interactions, such as those represented by the four-bodycyclic term
J
ring
, or even higher-order terms.The largest two-body couplings are expected to occur between NN sites although next-NN(NNN) interactions may be non-negligible or even of the same order of magnitude (cf CuGeO
3
system [26, 27]). Regarding the four-body operator terms, they may be important in Cu
4
O
4
plaquettes since their srcin lies in the cyclic circulation of electrons around the ring. Theirimportance and that of analogous cyclic six-body effects have been pointed out in other typesof half-ﬁlled band systems such as the
π
system of conjugated organic molecules [28]. Similarfour-body terms are crucial to describe the ground state properties of
3
He [29].The direct determination of the amplitude of the many-body terms of an extended spinHamiltonian such as the one in equation (2) from experiment is, in general, impossible. Spinladders with a variety of intersite distances represent an especially difﬁcult case. In general, theexperimental determination of the coupling constants is based on a series of hypotheses aboutthe negligibility of interactions between ‘remote’ sites. From these hypotheses, a given spinmodel is assumed and validated only from a numerical ﬁt of the thermodynamic or spectralproperties. It is customary to consider NN interactions only although this may be an excessivesimpliﬁcation and eventually can lead to contradictory estimates of the dominant couplings.This is precisely the case of the cuprate spin ladders for which conﬂicting values of the
J
rung
/
J
leg
ratios ranging from 0.5 to 1.0 were proposed. Interactions involving sites at a longer distance or
New Journal of Physics
9
(2007) 369 (http://www.njp.org/ )
4involving various sites had to be invoked to rationalize the different experimental results arisingfrom different techniques. One may think for instance in inter-ladder interactions, diagonalterms in the plaquettes or four-body cyclic effects. Indeed, several theoretical studies seem toconsistently indicate that four-body terms (
J
ring
) are crucial [21]–[24]. Here, it is important
to point out that very recently Toader
et al
[30] provided strong experimental evidence of the importance of the
J
ring
term in La
2
CuO
4
with
J
ring
≈
0
.
5
J
. This value is comparable tothe pairing energies and strongly suggests that the resulting circulating currents could have animportantroleinthemechanismofsuperconductivity.Thisisincontrastwithpreviousestimatesof
J
ring
for 2D and spin ladder cuprates, obtained either from indirect measurements or fromnumerical simulations with an extended Heisenberg model, which propose substantially smalleramplitudes with
J
ring
∼
0
.
3
J
[19, 21, 22, 24, 31]. The srcin of these discrepancies relies on the
choice made by different authors for the magnitude of the other coupling constants in the spinHamiltonian of equation (2). Hence, the
J
ring
term as evaluated by Toader
et al
relies on NNand NNN coupling constants of
J
=
111
.
8meV and
J
d
=−
11
.
4meV, respectively, extractedfrom one of the various ﬁttings of the magnon spectrum [22]. However, it is important topoint out that this value for
J
is smaller than another experimental estimate of 135
±
6meVobtained with a NN Heisenberg Hamiltonian [32]. Moreover, one should note that the presentestimate of a FM
J
d
differs from previous theoretical predictions [33] and from ﬁtting toexperimentalmeasurementsonmaterialswithsimilarexchangepaths[34].However,oneshouldalso recognize that the theoretical study by Annett
et al
[33], takes only into account two-electron processes to evaluate this
J
d
term while, as clearly explained by Toader
et al
[30]and references therein, the FM character of
J
d
arises precisely from three-electron exchangeprocesses around a plaquette, which are of the same order of magnitude as four-electronexchange processes around the same plaquette and which are not taken into account in [33, 34].
The discussion above illustrates the difﬁculties faced by experimentalists when attempting toextractthemagnitudeoftheimportanttermsandtheneedforindependentaccurateandunbiasedtheoretical predictions. For the SrCu
2
O
3
ladder compound a similar situation is encountered; therecent Raman response experiments by Schmidt
et al
suggest
J
rung
=
140meV,
J
ring
/
J
rung
=
0
.
2and
J
leg
/
J
rung
=
1
.
5 [35], in contrast with previous work indicating a more isotropic behaviorbetween rungs and legs [36].From the preceding discussion it is clear that an accurate prediction of the various magneticinteractions entering in the spin Hamiltonian as in equation (2) is not only highly desirable tounderstand the ground state properties of this kind of systems but urgently needed. One could,for instance, start from some approximate electronic Hamiltonian such as a single-band modelinvolving only the magnetic centers or a two-band model involving also the electrons of thebridging ligands. However, this is likely to introduce even more problems since it is difﬁcultto assess the accuracy of such a multiparametric approach. An alternative and straightforwardway to an unbiased estimate is the direct evaluation of the amplitude of the relevant magneticinteractions on a realistic model system treating all the electrons in a large enough basis set.If practicable, this pragmatic approach will present the advantage of providing an independent,unbiased and consistent prediction of the amplitude of relevant exchange parameters that cansolve the difﬁculties encountered by the usual ﬁtting techniques used by experimentalists.Unfortunately, the direct calculation of the important terms is not a simple task since italso requires the use of a model for the solid. In a ﬁrst approach, one may neglect translationalsymmetry and deﬁne a properly embedded ﬁnite cluster, a fragment of the periodic lattice withtwo, three or four magnetic sites with their coordination ligands and perform the best
ab initio
New Journal of Physics
9
(2007) 369 (http://www.njp.org/ )

Search

Similar documents

Tags

Related Search

A Linguistic Approach to NarrativeA Mirror Belonging to the Lady-of-UrukCulture as a Motivational Factor to Learn a FA new approach to denoising EEG signals-mergeMany-body Quantum ChemistryQuantum Many-Body PhysicsMany Body QuantumA Genre Approach to Syllabus DesignA Sociocultural Approach to Urban AestheticsA Systemic Approach to Leadership

We Need Your Support

Thank you for visiting our website and your interest in our free products and services. We are nonprofit website to share and download documents. To the running of this website, we need your help to support us.

Thanks to everyone for your continued support.

No, Thanks